Discussion Chain ID: 65862
================================================================================

User asked: Oxidation state of tungsten in W3O8

Recently I came across this equation: $$\ce{WO_3 +SnCl_2 +HCl\rightarrow W_3O_8 + H_2SnCl_6 +H_2O}$$ The compound $\ce{W_3O_8}$ that appears in the right hand side of the equation seems to be mixed oxide. Normal calculation of the oxidation state of W in the compound yields $\ce{\frac{16}{3}}$ which is a fraction. A google search on the compound does not give any good results too. So, is $\ce{W_3O_8}$ a mixed oxide? What are the oxidation states of the different tungsten atoms?

Discussion:
Comment: This might be helpful. https://www.researchgate.net/profile/Jun_Li36/publication/7378383_On_the_Structure_and_Chemical_Bonding_of_Tri-Tungsten_Oxide_Clusters_W_3_O_n_-_and_W_3_O_n_n_7-10_W_3_O_8_As_A_Potential_Molecular_Model_for_O-Deficient_Defect_Sites_in_Tungsten_Oxides/links/09e4150a75dbf3d339000000.pdf?origin=publication_detail
Comment: this http://dx.doi.org/10.1063/1.3505689 article claims that some 'extra' electrons on W are localized on specific atoms. So it seems that the compound *may* be classified as mixed oxide. However, it belongs to a weird family of Magneli phases, which are ... somewhat special. They are not non-stechiometric per se, but close to it. I'm not qualified enough to give a full conclusion, though.

Answer 1 (5 votes):
**TL; DR** : If you are forced to list the formal oxidation states, then with a high level of confidence it's tungsten(V,VI) octaoxide $\ce{W^{VI}W^V2O8}$. However, the real product of this reaction would be a number of non-soichimetric tungsten(IV,V,VI) oxides. Formation of molecular oxoclusters or peroxo compounds is very unlikely. * * * Reduced tungsten oxides are generally non-stoiciometric. Glemser et al. [[1](https://doi.org/10.1002/zaac.19643320511)] reduced tungsten(VI) oxide hydrates $\ce{WO3 * H2O}$ and $\ce{WO3 * 2 H2O}$ with $\ce{Zn}$ in $\ce{HCl}$ to the blue tungsten oxide hydrates of the general formula $\ce{WO_{3‐x}(OH)_x}$ $(x → 0.5)$ with the lowest reducing degree of $2.65$, which is very close to the one in $\ce{W3O8}$ $(8/3 = 2.6(6))$. I would expect that $\ce{SnCl2}$ in acidic media would have comparable reducing effect. With the moderately mild reducing agent such as tin(II) chloride there is very little chance of ending up exclusively with $\ce{W3O8}$. Also, a presence of a reducing agent also eliminates a possibility of the formation of the peroxo-compounds, so that with a high level of confidence we are dealing with oxide $\ce{O^2-}$ ligand. I find it equally improbable that any cluster formation takes place. For the existence of a polyoxotungstate cluster the terminal $\ce{W=O}$ bonds must be "disarmed" in order to prevent further olation/oxolation and aggregation into bulk metal oxide. This is often achieved via the template effect, however even reduced by 1 to 6 electrons forms of 12-heteropolytungstates $\ce{[(P,Si)W12O40]^3-}$, the phosphate- or silicate-templated Keggin structure — one of the most stable — only exist briefly in solution [2, pp. 341–343]. In the presented system there is no suitable anion to preserve the three-membered $\ce{W3O8}$ ring, and it's very likely going to hydrolyze quickly. To sum these thoughts up, the more appropriate way to write the reaction would be $$\ce{n WO3 + SnCl2 + 4 HCl → W_nO_{3n-1} + H2SnCl6 + H2O}$$ where $\ce{W_nO_{3n-1}}$ is homologous series analogous to the mixed-valence tungsten blues. On crystallographic level this can be seen as withdrawal of oxygen atoms from $\ce{WO3}$, which is isostructural to [$\ce{ReO3}$](https://en.wikipedia.org/wiki/Rhenium_trioxide) (Fig. 1a). New point defects are eliminated by introducing a crystallographic shear (CS, Fig. 1b). As the reduction proceeds, the octahedra $\ce{[WO6]}$ in this structure changing from corner-sharing to edge-sharing motif (Fig. 1c). (Caption and adapted illustration from [3, p. 1086].) > [](https://i.sstatic.net/kkDZr.png) > > **Figure 1.** Crystallographic shear in $\ce{WO3}$ (**a**) the idealized structure of $\ce{WO3}$, drawn as corner-shared $\ce{WO6}$ octahedra, squares in projection (**b**) {102} CS planes (arrowed), consisting of blocks of four edge-shared octahedra (**c**) {103} CS planes (arrowed), consisting of blocks of six edge-shared octahedra. It's impossible to deduce exact oxidation number for such structure with floating stoichiometry, but sure enough an _average oxidation number_ of tungsten can be found trivially from the $\ce{W_nO_{3n-1}}$ formula: $$\text{O.N.}(\ce{W})\cdot n - 2(3n - 1) = 0 \qquad\to\qquad \text{O.N.}(\ce{W}) = 6 - 2/n,$$ e.g. for $\ce{W3O8}$ $\text{O.N.}(\ce{W}) = 6 - 2/3 = 5.3(3)$. Boundary case $n = 1$ dictates the lowest $\text{O.N.}(\ce{W}) = 4$, so that $\ce{W_nO_{3n-1}}$ phase consists of a mixed-valence oxide with various ratios of $\ce{W(VI)}:\ce{W(V)}:\ce{W(IV)}$. Exact ratio is to be determined from [XPS](https://en.wikipedia.org/wiki/X-ray_photoelectron_spectroscopy)/[XANES](https://en.wikipedia.org/wiki/X-ray_absorption_near_edge_structure) analysis for a given specimen; spectrophotometry would be difficult to implement as tungsten oxides have negligible solubility in most solvents unless some peroxide or $\ce{HF}$ is added. Exact location of the reduced tungsten centers can be averaged by finding CS areas with [EM](https://en.wikipedia.org/wiki/Electron_microscope)/[PXRD](https://en.wikipedia.org/wiki/Powder_diffraction) analysis. Now, to the $\ce{W3O8}$. In fact, it's already been synthesized by Zakharov et al. as follows [[4](https://doi.org/10.1107/S0108768193005701)]: > The sample examined was prepared by partial reduction of $\ce{WO3}$ with carbon at high temperature in combination with high pressure. The reaction occurred between the graphite container material and a pressed tablet of $\ce{WO3}$ in a closed system ($T = \pu{1773 K}$, $P = \pu{50e5 kPa}$). [...] The product obtained was a mass containing minute dark-red crystallites. The colour suggested that considerable reduction had taken place. and two phases were characterized with EM/PXRD. Authors also suggest that $\ce{W3O8}$ can hardly be obtained under ambient conditions: > The two phases, both of composition $\ce{W3O8}$ $(\ce{WO_{2.667}})$, do not appear in the binary $\ce{W-O}$ system at ambient pressure. $\ce{W3O8(I)}$ has a structure of the $\ce{U3O8}$ type (Andresen, 1958), which is denser than that of $\ce{W3O8(II)}$. The latter has a new type of structure, although some features are shared with other previously known tungsten oxides ({102} CS structures). [](https://i.sstatic.net/KxgDp.png) **Figure 2.** Idealized polyhedral representation of $\ce{W3O8(I)}$ [](https://i.sstatic.net/ca5Pw.png) **Figure 3.** Idealized polyhedral representation of $\ce{W3O8(II)}$ So, there are two possible combinations for the formal $\text{O.N.}$s: 1. $1~\ce{W(VI)} + 2~\ce{W(V)}$; 2. $2~\ce{W(VI)} + 1~\ce{W(IV)}$. Unfortunately, oxidation states are not mentioned in the article and I haven't found any citeable sources with the determination of oxidation numbers for $\ce{W3O8}$, but the XPS studies of [uranium octaoxide $\ce{U3O8}$](https://en.wikipedia.org/wiki/Triuranium_octoxide) indicated the presence of two oxidation states, $\ce{U(VI)}$ and $\ce{U(V)}$, in a $1:2$ ratio, respectively. Since phase $\ce{W3O8(I)}$ is isostructural, there is a high chance that the scenario 1, $1~\ce{W(VI)} + 2~\ce{W(V)}$, is quite plausible. Having the CIFs of both structures at hands, I've been trying to perform bond-valence analysis, but with the [common tabulated empirical parameters](https://www.iucr.org/resources/data/datasets/bond-valence-parameters) I haven't reached any meaningful results. Mixed-valenced tungsten and molybdenum oxides often contain delocalized $\mathrm{d}$ electrons, making bond-valence analysis alone less meaningful [[5](https://doi.org/10.1016/0022-4596\(85\)90256-7)]. ### References 1. Glemser, O.; Weidelt, J.; Freund, F. Genotypische Oxidhydrate des Wolframs. Zur Frage der Wolframblauverbindungen. _Zeitschrift für anorganische und allgemeine Chemie_ **1964** , 332 (5–6), 299–313. <https://doi.org/10.1002/zaac.19643320511>. 2. Advances in Inorganic Chemistry and Radiochemistry; Emeléus, H. J., Sharpe, A. G., Eds.; Advances in inorganic chemistry and radiochemistry; _Academic Press: New York_ , **1967** ; Vol. 10. ISBN 978-0-08-057859-0. 3. Encyclopedia of Inorganic Chemistry, 2nd ed.; King, R. B., Ed.; _Wiley: Chichester, West Sussex, England ; Hoboken, NJ_ , **2005**. ISBN 978-0-470-86078-6. 4. Sundberg, M.; Zakharov, N. D.; Zibrov, I. P.; Barabanenkov, Y. A.; Filonenko, V. P.; Werner, P. Two High-Pressure Tungsten Oxide Structures of $\ce{W3O8}$ Stoichiometry Deduced from High-Resolution Electron Microscopy Images. _Acta Crystallographica Section B Structural Science_ **1993** , 49 (6), 951–958. <https://doi.org/10.1107/S0108768193005701>. 5. Domenge`s, B.; McGuire, N. K.; O’Keeffe, M. Bond Lengths and Valences in Tungsten Oxides. _Journal of Solid State Chemistry_ **1985** , 56 (1), 94–100. <https://doi.org/10.1016/0022-4596(85)90256-7>.


================================================================================

